SUPERSEDED (click for Active standard)
| ||Format||Pages||Price|| |
|6||$62.00||  ADD TO CART|
1.1 This test method covers the determination of the microindentation hardness of powder metallurgy (PM) materials. The test method differs from the approach used for pore-free materials in terms of the precautions required to deal with the porosity.
1.2 This procedure covers tests made with the Knoop or Vickers indenters under loads in the range from 1 to 200 gf.
1.3 Automated testing is not generally suitable for use with porous PM materials, because acceptable indentations require avoiding placing indentations in the immediate vicinity of a pore, a condition not guaranteed with automated placement of the indentations. Any automated testing shall allow for review of indentations post-test to reject any distorted or unusually large indentations in accordance with .
1.4 A method for converting the directly measured indentation lengths to other hardness scales, for example, HRC is described in .
1.5 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B243 Terminology of Powder Metallurgy
E384 Test Method for Microindentation Hardness of Materials
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
MPIF StandardsStandard 70 Guide to Sample Preparation of Ferrous Powder Metallurgy (PM) Materials for Cross-Sectional Metallographic Evaluation Standard 71 Guide to Sample Preparation of Copper-Based Powder Metallurgy (PM) Materials for Cross-Sectional Metallographic Evaluation Standard 72 Guide to Sample Preparation of Aluminum Powder Metallurgy (PM) Materials for Cross-Sectional Metallographic Evaluation
ICS Number Code 77.160 (Powder metallurgy)
UNSPSC Code 31133700(Powdered metals and metal alloys)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM B933-16, Standard Test Method for Microindentation Hardness of Powder Metallurgy (PM) Materials, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top